STANSLAUS MANYENGO LUSAMBILI, BEd (Sc)
Reg. No. I56/24068/2012
A Thesis Submitted in Partial Fulfillment of the Requirements for the Award of the Degree of Master of Science (Chemistry) in the School of Pure and Applied Sciences of Kenyatta University
I declare that this thesis is my original work and has not been presented for a degree or
any other award in any other university/institution.
Signature ……… Date ……… Stanslaus Manyengo Lusambili
We confirm that the work reported in this thesis was carried out by the candidate under our supervision and has been submitted with our approval as university supervisors.
Dr. Evans C. Ogwagwa Department of chemistry Kenyatta University
P.O Box 43844-00100 Nairobi
Signature……… Date ………
Dr. Alphonse W. Wanyonyi, Department of chemistry Kenyatta University
P.O Box 43844-00100 Nairobi
To my father, the late Samuel Shikundi Lusambili and my mother Veronika Achekulwa
Lusambili for sacrificing about all they laid their hands on for my education. I also dedicate this thesis my wife Victoria Sheila Lusambili, my daughters; Petronila
My special thanks go to my supervisors Dr. Evans C. Ogwagwa and Dr. Alphonse W.
Wafula for tirelessly directing and guiding me throughout the collection of data and writing of this thesis. I express my gratitude to all the teaching and non-teaching staff at
Chemistry Department, Kenyatta University, for their assistance throughout this course.
I acknowledge the laboratory staff in the Chemistry and Civil Engineering departments of
Jomo Kenyatta University of Agriculture and Technology, the directors of; Roads Transport and Infrastructure Research laboratory, ICRAF, KEBS and KALRO for
allowing me to use their facilities for sampling and testing.
May I also sincerely thank Wycliffe Atinya Shisundi and Josephat Makomere Mukhaya
of the Ilesi Traditional Pottery for supplying me with their mixtures of molded clays and facilitating the acquisition of the raw clays.
I thank the Government of Kenya through Teachers Service Commission for granting me three months study leave without which it would have been very difficult to collect data.
TABLE OF CONTENTS
ACKNOWLEDGEMENT ... iv
LIST OF TABLES ... ix
LIST OF FIGURES ... x
ABBREVIATIONS AND ACRONYMS ... xi
ABSTRACT ... xii
CHAPTER ONE ... 1
1 INTRODUCTION ... 1
1.1 Background information ... 1
1.2 Problem statement and justification of study ... 3
1.3 Hypothesis ... 3
1.4 General objective ... 3
1.5 Specific objectives ... 4
1.6 Significance of study ... 4
1.7 Scope ... 4
CHAPTER TWO ... 5
2 LITERATURE REVIEW ... 5
2.2 Classification of clays ... 5
2.2.1 Kaolins ... 6
2.2.2 Illites ... 7
2.2.3 Smectites ... 8
2.2.4 Palygorskite-Sepiolite ... 9
2.3 Composition of clays ... 10
2.4 Naming of clays ... 11
2.5 Pottery making process ... 11
2.6 Important characteristics of clays ... 12
2.6.1 Physical characterization ... 13
2.6.2 Analytical instruments ... 17
CHAPTER THREE ... 19
3 MATERIALS AND METHODS ... 19
3.1 Study site ... 19
3.2 Sample Collection and preparation. ... 20
3.3 Pretreatment of samples ... 20
3.3.1 Pretreatment for chemical characterization ... 21
3.3.2 Pretreatment for physical characterization ... 22
3.4 Physical parameter determination ... 23
3.4.2 Particle size analysis ... 25
3.4.3 Loss on ignition... 26
3.4.4 Moisture content ... 26
3.4.5 Shrinkage limits ... 27
3.4.6 Density ... 27
3.4.7 Porosity ... 28
3.4.8 Compressive strengths ... 29
3.5 Recipe formulation ... 29
3.5.1 Shrinkage limits ... 30
3.5.2 Density ... 30
3.5.3 Porosity ... 31
3.5.4 Compressive strengths ... 32
3.6 Losses ... 32
3.7 Data analysis ... 33
CHAPTER FOUR ... 34
4 RESULTS AND DISCUSSION ... 34
4.1 Introduction ... 34
4.2 Screening tests of raw clays ... 34
4.3 Mineral and chemical composition of raw clays ... 35
4.3.2 X-Ray Diffraction (XRD) ... 39
4.3.3 EDX spectroscopy ... 43
4.4 The Physical Properties of the Ilesi Clays ... 45
4.4.1 Plasticity index ... 45
4.4.2 Particle size analysis ... 47
4.4.3 Loss on ignition... 51
4.4.4 Moisture Content ... 52
4.4.5 Linear shrinkage... 54
4.4.6 Density ... 60
4.4.7 Porosity of fired clay bodies ... 63
4.4.8 Compressive strength ... 67
4.4.9 Losses ... 71
CHAPTER FIVE ... 74
5 CONCLUSIONS AND RECOMMENDATIONS ... 74
5.1 Conclusions ... 74
5.2 Recommendations ... 74
5.3 Recommendation for further work. ... 75
REFERENCES ... 76
LIST OF TABLES
Table 2.1: Examples of clay minerals ... 6
Table 2.2: Some clays with their percentage compositions ... 10
Table 2.3: Mineralogy of local clays in a Saudi Arabia ... 10
Table 3.1: Ratios of percentage raw materials by mass ... 30
Table 4.1: Sample groups ... 34
Table 4.2: Profile description of clay soils from deposit depths when milled ... 35
Table 4.3: Spectral bands and their assignments ... 39
Table 4.4: XRD data for the clay samples ... 39
Table 4.5: Percentage oxides of raw materials ... 43
Table 4.6: Atterberg limits for the black, brown and grey soils ... 46
Table 4.7: Soil texture ... 50
Table 4.8: Loss on ignition ... 51
Table 4.9: Percentage Moisture content... 53
Table 4.10: Linear dry and fired shrinkage from pure clays and clay mixtures ... 55
Table 4.11: Mean densities of dry and fired clay bodies ... 60
Table 4.12: Porosities of fired clay bodies ... 63
Table 4.13: Compressive strengths of green and fired clay bodies ... 67
Table 4.14: Losses incurred using shrinkage tests ... 71
LIST OF FIGURES
Figure 2.1: Diagramatic structure of kaolinite ... 7
Figure 2.2: Diagramatic structure of illite ………...8
Figure 2.3: Diagramatic structure of montmorillonite ………9
Figure 3.1: Map showing Ilesi clay deposit study site ... 19
Figure 4.1: FTIR spectrum for black clay ... 36
Figure 4.2: FTIR spectrum for brown clay ... 36
Figure 4.3: FTIR spectrum for grey clay ... 37
Figure 4.4:X-Ray Diffractogram for black clay ... 40
Figure 4.5: X-Ray diffractogram for brown clay soil ... 41
Figure 4.6: X-Ray Diffractogram for grey clay ... 42
Figure 4.7: Penetration against moisture content for the black, brown and grey clays .... 46
Figure 4.8: Percentage particles against diameter/mm for black soil ... 48
Figure 4.9: Percentage particles against diameter/mm for brown soil ... 49
Figure 4.10: Percentage particles against diameter/mm for grey soil ... 50
Figure 4.11: Shrinkage of dry and fired clay bodies ... 59
Figure 4.12: Densities of dry and fired clay bodies ... 62
Figure 4.13: Porosity of fired clay bodies ... 66
ABBREVIATIONS AND ACRONYMS
ANOVA Analysis of variance
ASTM American Society for Testing and Materials
CEC Cation exchange capacity
EDX Energy dispersive X-ray spectroscopy
FTIR Fourier Transform Infra-Red
ICRAF International center for Research in Agroforesty KALRO Kenya Agriculture Livestock Research Organization
KEBS Kenya bureau of standards
LOI Loss on ignition
SEM Scanning electron microscopy SCBA Sugarcane baggase ash
INTRODUCTION 1.1 Background information
Ilesi traditional pottery was started at Ilesi market, which is situated 5 km from
Kakamega town on the Kakamega- Kisumu road in 1963 (Amadala, 2013). The potters majorly fabricated water cooling pots for sale during market days at neighboring market centers. The activity has since grown into a cottage industry around Ilesi that makes
approximately 20,000 pot products in a month, directly and indirectly employing approximately 1,000 people. Search in the literature reveals no information about
characterization of the clays under use as much as they have been used for years. Furthermore, the users report losses due to breakages before and during firing of their products. This concern prompted a systematic study of the clays to determine their
characteristics and hence the suitability for pottery.
Clay is a natural resource used in the manufacture of a number of products among them, fired bricks, refractory bricks, tiles, deep well drilling mud, biomedical implants, manufacture of paper and paints, tobacco pipes and pottery (Adelabu, 2012). Its usage for
current and new applications will continue to grow since it is a cheap and environmentally friendly raw material. Most table wares like pots, urns, utensils, pestles,
mortars are made from earthen clays. Applications and uses of clays in ceramics depend on their chemical and physical properties like plasticity, moisture content, porosity, particle size, shrinkage, firing temperature, strengths of structure, structure of clay,
Pottery making involves molding and mixing raw materials, forming, drying and firing of the product. The potters at Ilesi follow these steps. They mix the black, brown, and grey
clays in equal quantities. They add grog sand measuring half of the clay ratios by mass to the clay mixture. They use traditionally made kilns whose firing temperatures cannot be
altered much (Gosselain, 1992) but have enabled them to remain in production. The potters however, still make some losses due to breakages in the process of forming and firing however losses due to kilning techniques are reduced by training and gaining
experience in the art (Gossenlain, 1992). Pot making business can be improved by training and innovation which influences access to new markets.
The marketing is dominated by middle men who source pots especially for urban and tourist markets. The techniques that alter the visual and tactile characteristics of pottery
correspond to the economic situation of the potters, their age and broad interaction networks through which their goods are consumed (Gosselain, 2000).
Clays for pot-making should have plasticity index of between 15-25% (Abuh, 2004; Allen, 1986; Wanyonyi, 2004), a porosity of 4-10% (Kirabira, 2003; Nweke, 2007),
shrinkage of 4-17% (Allen, 1986; Kirabira, 2003), firing temperature of 700-1100°C (Bordeepong et al; 2012; Maggate et al., 2010), fired strengths of 27 to 70 MPa (Allen,
1.2 Problem statement and justification of study
Pottery in Kakamega County, is largely done through non-conventional methods. The
clays have not been characterized and the recipe they use is not recorded but handed down orally and by practice from generation to generation making reproducibility
impossible. The potters incur losses of between 20% and 30% due to swelling of clays during molding, cracking of pots during drying and breakages during firing. It is not clear whether these losses are due to the unsuitability of the clays or the handling of it during
the production process. This study therefore, sought to characterize the Ilesi clays by determining their suitability in terms of requisite physical properties such as Atterberg
limits, porosity, shrinkage limit, clay content, moisture content, clay body density, particle size, loss on ignition and pressure of rupture. It also sought to determine the most suitable method as well as mixing ratio for best results.
The clays used for pot making in Kakamega County are suitable for pottery but are not handled appropriately.
1.4 General objective
To characterize and determine the suitability of the raw clays and recipe used by Ilesi
1.5 Specific objectives
i). To determine the mineral content of Ilesi clays using X-Ray Diffraction
ii). To determine the elemental composition of the clays and grog sand using Energy
Dispersive X-Ray Spectroscopy (EDX).
iii). To determine the physical properties (plasticity index, porosity, shrinkage limit,
loss on ignition, compressive strengths, sieve analysis, density and moisture
content) of the raw clays used, Ilesi mixture and formulated clay mixtures.
1.6 Significance of study
The study will document clay mineral quantities in the raw clays and their suitability for pottery making which will contribute to the clay literature in the county and county. The
characterization will reveal what else the clays are suitable for and possibly spur diversification of products produced. The results may boost consumer confidence for
importers and reduce poverty due to improved sales.
2 LITERATURE REVIEW
Potters use raw clays for making ceramic pots. In most cases they do this without
knowledge of the basic characteristics of clays for this purpose (Amponsah-Dacosta et al., 2013). This is not different to the potters at Ilesi who have used their raw clays for pottery over five decades.
2.2 Classification of clays
Clay is a natural, earthy and fine grained material comprised of a group of crystalline minerals known as clay minerals (Kirk and Othmer, 2004). They are generally plastic at appropriate water contents and will harden when dried or fired (Mukherjee, 2013). Flint
clays and halloysites are however not plastic (Grim, 1962).
Clays are classified into Kaolins, Smectites, Mica, Serpentite, Vermiculite, Sepiolite and Pylophylite (Guggenheim and Martin, 1995). They are formed from hydrolysis and hydration of silicates, dissolution of limestone rocks, slaking and weathering of clay rich
sedimentary rocks and as a product of hydrothermal decomposition of granite rocks (Lee, 1986). The feldspars in granite rocks decompose over very many years to yield kaolins,
silica and potash or soda as shown by the equations (1) and (2) below.
When the KOH and NaOH formed dissolve due to effects of rain, the remaining clay minerals form kaolins that exist in four different structures, kaolinite, dickite, nacrite and
halloysite, a hydrated analogue (Kirk and Orthmer, 2004). The other clay minerals like smectites, serpentines, illites and sepiolites are formed when some of the aluminium in
the structure is replaced by magnesium, iron, calcium, or lithium (Bohn et al., 2001). Kaolins are coarse, with a particle size of 2.0-3.0 m while smectites and micas have fine
texture and particle sizes of below 0.5 m (Heckroodt, 1991). Table 2.1 gives a list of some of the clays discussed below (Kirk and Orthmer, 2004).
Table 2.1: Examples of clay minerals
Clay Clay mineral Formula
Kaolins Kaolinite Al2O3.2SiO2.2H2O Dickite Al4Si4O10(OH)8 Nacrite Al2O3.2SiO2.2H2O Halloysite Al2O3.2SiO2.4H2O
Mica Illites Ky(Al4Fe4.Mg4Mg6)(Si8-y)O20(OH)4 Smectites Montmorillonite Al1.67Mg0.33(Na0.33)Si4O10(OH)2
Beidellite Al2.17 [Al0.33(Na0.33)Si3.17]O10 (OH)2 Nontronite Al2.17 [Al0.33(Na0.33)Si3.67]O10 (OH)2 Fuller’s earth Palygorskite-Sepiolite (Mg, Al)Si4O10.4H2O
Kaolins are white to grey plastic clays formed by alteration of feldspar and muscovite.
Whereas the primary kaolins result from residual weathering or hydrothermal alteration of silicates the secondary ones are formed by flow (Bohn et al., 2001). Kaolin
polymorphs can only be distinguished by x-ray diffraction spectroscopy, XRD (Edward et al., 1976).
down which explains their low plasticity, shrinkage and swelling properties (Tan, 2011). The Kaolin sheets are held together by hydrogen bonds that prevent expansions which
also prevents entry of polar molecules hence a very low cation exchange capacity (CEC) of 10 to 100mmolkg-1 (Bohn et al., 2001). Figure 2.1 shows the structure of a kaolinite
Figure 2.1: Diagramatic structure of kaolinite
Kaolins are the most widely used clays since they are pure and have high brightness, relatively low viscocity at high concentration (Sposito, 1989). They are used in pottery,
manufacture of plastics, rubber, paint, cement among others.
Illite is a general term for clay constituents or argillaceous sediments that belong to
hydrous mica group. It is a significant rock forming mineral being a main component of shales and other argillaceous rocks with a formula, (K,H)Al2(Si,Al)4O10(OH)2.xH2O,
Hayes, 1991). Figure 2.2 shows the structure of Illite with K+ distributed within the inter layer (en.wikipedia.org).
Figure 2.2: Diagramatic structure of illite
Smectites are clay minerals that carry a lattice charge and usually expand when solvated with water or alcohol. Their 2.1 structures are arranged in silica-gibbsite- silica lattices. The aluminium in the Al(OH)3 sheet is heavily substituted by iron and magnesium which
gives the sheet a negative charge (Gieseking, 1975). Smectites have very small particle size with high affinity for water hence very plastic. They have low layer charge that
causes a lot of isomorphic substitutions. The weak forces of attraction between crystal lattice enables polar molecules like water to enter the inter layer. This causes the clays to readily expand. The c-spacings are between 0.95 to 1.0 nm with high degree of interlayer
montmorillonite, beidellite and nontronite. They are usually used as metal ion adsorbents due to the negative charge. They are used in drilling muds, ceramics, foundry binders,
sealants, iron ore pelletizer, adsorbents etc. Figure 2.3 shows the structure of montmorillonite indicating the position of magnesium and iron (II) on the octahedral
Figure 2.3: Structure of montmorillonite
Both palygorskite/attapulgite and sepiolite are hydrated magnesium, aluminium silicates of elongated chain structures. Sepiolite, however has higher magnesium content and large
unit cell than palygorskite. These clays do not flocculate with electrolytes and are stable at higher temperatures, a property that determines their uses (Murray, 2002) like drilling
2.3 Composition of clays
The chemical substitution of aluminium by silicon, iron(III) and/or magnesium in clays
generates positive and negative charges on the structure causing variations in the compositions of clays (Garrison, 1989). These compositions of clays vary in the minerals
in which they occur. Clays exist in two structural sheets 1.1 that is gibbsite sheet Al(OH)3 or (Mg(OH)2)/ silicate sheet (SiO2) as in kaolinite and the 2.1, which is a silicate sheet / gibbsite sheet /silicate sheet (Lee, 1986) as in smectite (Grimshaw, 1971; Kirk and
Othmer, 2004). Table 2.2 shows compositions for some pure clay minerals (Grimshaw, 1971).
Table 2.2: Some clays with their percentage compositions
Clay SiO2 Al2O3 Fe2O3 TiO2 CaO MgO Na2O K2O Kaolinite 45.44 38.52 0.30 0.16 0.08 0.08 0.66 0.14 Illite 51.22 25.91 4.59 0.53 0.16 2.84 0.17 6.09 Allophane 32.30 30.41 0.23 0.0 0.10 0.29 0.0 0.0 Montmorillonite 51.14 19.76 0.83 0.0 1.62 3.22 0.04 0.11
This data shows that clays have high percentage compositions of SiO2, Al2O3 and low percentage composition of Fe2O3, CaO, Na2O, TiO2 and K2O. Most clay deposits are found as mixtures of clay minerals or a clay mineral in presence of other minerals. Table
2.3 shows percentage compositions of raw clays in Saudi Arabia (Mohsen and El-maghraby, 2010).
Table 2.3: Mineralogy of local clays in a Saudi Arabia
Raw clay Kaolinite Illite Quartz Montmorillonite Albite Haematite
%White Clay 0 0 45 50 0 5
%Red Clay 40 0 18 12 16 14
2.4 Naming of clays
Clays are complicated to name and therefore they are given names that are indicative
i) pot clays for those that are used for pottery,
ii) china clay are usually plastic and give dense fired body,
iii) ball clays are plastic clays that burn into white material, they have very fine grain
size and high plasticity,
iv) refractory clays are clays with high resistance to heat without loss of shape and
v) flint clays are virtually non plastic ones (Allen, 1986; Glenn and Burkett, 2002).
2.5 Pottery making process
Pottery making is usually carried out in six stages, acquisition of raw materials, clay
processing, pot shaping, pot decoration, firing and post pot treatments like painting, application of water proofing resins (Kent, 2008). The number of steps taken by potters
depends on their underlining cultures and market forces. Potters mix raw materials in ratios such as to improve the quality of their products and workability of the clay body. For example potters at Ilesi use equal ratios of the black, brown, grey clays and half grog
sand while those at lower Thukela in KwaZulu-Natal prefer ratios of 60:40 and 50:50 black to red respectively (Kent, 2008).
grog, a coarse alumina, silica ceramic material. The filler reduces shrinkage and aids even drying.
Ceramics are made into paste and shaped at normal temperatures (Grimshaw, 1971).
Firing gives them strength either by sintering crystallites together or partly melting them into a paste. The firing temperature range from 100°C to 1775°C causes changes in minerals or crystal phase through thermal expansion or shrinkage (Heimann and Franklin,
1979). The firing temperature also affects the color of the pot. A red colour shows an oxidizing atmosphere while black or grey indicates either insufficient firing time or
reducing atmosphere (Tite, 2008). Firing at higher temperatures more than 1100°C vitrifies the clay by glazing the material increasing mechanical strength in addition to aesthetic effects.
Potters process clay to improve plasticity, workability and thermal shock resistance
(Bronitsky and Hammer, 1986; Skibo et al., 1989). By mixing different types of clays in different proportions and combinations, potters are able to make many products (Rusovich-Yugai and Neklyudova, 2007). Some researchers have mixed their clays with
waste materials like ground glass or sugarcane baggase ash, SCBA as fillers (Tonnayopas, 2013) and formed pots.
2.6 Important characteristics of clays
Some of the physical characteristics that determine use of clays for pottery are plasticity,
three major ways of characterizing clays in order to determine their uses, namely physical characterization, use of organic stain reactions and use of analytical instruments.
2.6.1 Physical characterization
In this characterization, the physical parameters listed below are determined and then compared with data in literature.
126.96.36.199 Plasticity Index
Plasticity is the property of clay such that when mixed with sufficient amount of water undergoes deformation by application of slight pressure and retention of the deformed
shape after release of the pressure (Ghildyal and Tripathi, 1986). Some researchers have used values of plasticity index to characterize clays (Amponsah et al., 2013). In this
characterization the plastic and liquid limits are determined which indicate the range of workability of clay body. A plot of plastic limit on x-axis against plasticity index can be used to identify clay minerals (Bain, 1971). Clays with large particle size like kaolins
have lower plasticity. Their structures have smaller water absorption capacity. Plastic and liquid limits are measured as percentage water that makes a soil plastic or liquid
respectively. The plasticity index is determined as a ratio of the liquid and plastic limits. A plasticity index of 15 to 25% is considered suitable for pottery making.
Shrinkage is the contraction of a clay body on drying or firing. Shrinkage depends largely
shrinkage effects. Linear shrinkage is measured as percentage contraction in millimeters. It is important because it determines the dimensions of a wet pot. Large and rapid
shrinkage during drying and firing is one of the causes of pot breakages (Allen, 1986).
Porosity is a measure of empty space in a soil material as a fraction to the total volume. It describes the fraction of voids or pores in a material. These are the empty spaces in a
material where water can reside in a soil.
Porosity of a soil generally increases with increase in particle size. Kaolins have large porosity due to their large particle size hence low plasticity. They are preferred for pottery but for very plastic clays like most smectites, tempers are added to enable them
allow water to dry out without cracking. Kaolinite occurs largely as discrete particles mainly in form of pseudo-hexagonal sub-idiomorphic platy crystals loosely attached to
the walls of pores (Morris and Shepperd, 1992). This cornflake arrangement produces extensive micro pore space. Entrapment of water results into static permeability reduction and is caused by clay expansion both within the structure and by increased separations of
individual particles, this results into restriction and blocking of pore throats.
of the smaller particles dissolve. Beyond this, vitrification proceeds and porosity decreases to theoretical zero at 1220°C.
Porosity is determined by measuring the amount of water a fired clay body absorbs over a
period of time. This parameter depends on duration of the soaking of the pot into water and hence its standards vary from country to country.
188.8.131.52 Compressive strength of clays
Strength of a clay body is associated with the effects of the hydroxyl of water either
through cohesion forces or reactions with elements in the structures. Compressive strengths or modulus of rupture represent the amount of load a body can hold without breaking (Parashar and Parashar, 2012). It depends on the forces of attraction between the
sheets and layers in the clay minerals. It is influenced by the water and accessory ions in the interlayer, c-spacings and type of clay mineral lattice (Ding et al., 2001). Fired
strength increases with firing temperature due to increase in crystal forms that increase the surface tension forces (Agbalajobi and Omoijuanfa, 2012). It is measured as a crushing force per unit area in MPa (Mbereyaho and Twubahimana, 2013).
The density of a clay body is the ratio of its mass to its volume. The densities of clay bodies increase with increase in temperatures of the clay bodies. The glass formation continues to increase the density until its maxima though this maxima is practically close
Glass undergoes a glass transition within a range of temperatures in which physical properties like density, viscosity, heat capacity, porosity are changed reversibly by
appropriate heat treatment (Thompson, 1995).
As the clay crystal phase changes between 1000°C to 1250°C, the Na2SiO3(l) formed according to equation (3) below flows into the interlayer distances filling the pores exposing the sheets directly to the charge difference attractions that makes the structure
Na2O(s) + SiO2(s) →Na2SiO3(l) Equation (3)
184.108.40.206 Loss on ignition
Loss on ignition (LOI) is widely used to estimate the amount of organic carbon and
inorganic carbon in the soil (Dean, 1974). This method is based on differential thermal analysis in which organic matter begins to ignite at 200°C and burns out by 550°C
(LOI550) while most carbonate minerals that represent the inorganic carbon are destroyed at higher temperatures of 850°C for calcite and 750°C for dolomite depleting at LOI950 (Goldin, 1987). The calculation of the carbon matter burnt out of the sediment assumes
that the ignition follows a stoichiometric relationship (Juan et al., 2004). However some non carbon materials like phosphorus and sulphur in the sediments reduces the
2.6.2 Analytical instruments
There are a number of analytical instruments used in characterization of clay minerals. The instruments are selected according to need and availability. Some of the instruments used are:
220.127.116.11 X-Ray Diffractometry (XRD)
XRD disperses a crystal lattice using an x-ray beam and identifies the material by measuring the d-spacings and degrees, 2 of diffracted x-ray beamaccording to Bragg’s
law, 2dsin =λ (Weitkamp et al., 2005). The diffracted x-ray beam is detected as a
characteristic x-ray line on photographic plates. The measured line through Fourier Transform is compared to a catalogue of known substances.
However due to the irregular and complex nature of the clay mineral lattice especially in
common clays XRD peaks do not resolve well. The collected data may substantially vary from sampled standards. It is therefore important to correlate the data received with an FTIR spectrum of the clay body.
18.104.22.168 Fourier Transform Infrared Spectroscopy (FTIR)
An IR radiation is passed through a sample from a glowing black-body source. Part of the radiation passes through while part is absorbed so long as the molecule has dipole moments. The irradiation causes vibrations, bending and/ or stretching of the molecular
bonds whose frequencies are detected producing a spectrum that represents molecular absorption or transmittance as a unique molecular fingerprint. This analysis identifies
digitalized and sent to the computer where Fourier transformation takes place. This technique is nondestructive, is a high speed determination with increased sensitivity and
measures all frequencies simultaneously due to the interferometer.
22.214.171.124 Energy Dispersive X-ray Spectroscopy (EDX)
Energy Dispersive X-ray spectroscopy relies on the interaction of the sample and some x-ray excitation. A high energy beam of electrons, protons or a beam of x-x-ray is focused
onto a solid sample. The incident beam of electrons may excite and eject an electron from an inner energy shell creating an electron hole. An electron from a higher energy level
3 MATERIALS AND METHODS
3.1 Study site
Ilesi in Kakamega County is situated on latitude 0.28° N and longitude 34.75°E. The
study targeted three clay types and a grog sand used by the Ilesi potters in Shinyalu subcounty, 4 km south of Kakamega town, along the Kisumu to Kakamega road. Sugarcane baggase ash (SCBA) from Butali Sugar factory which is 20 kms north-east of
Kakamega town was also collected and used in one of the mixtures in a bid to determine its possible inclusion in pottery. Figure 3.1 shows map of sites of study.
3.2 Sample Collection and preparation.
Purposive sampling was used on the known Ilesi clay deposit sites (Christine, 2013). The
area of about an acre along the swampy stream was marked with assistance of a member of the Ilesi traditional pottery. A pit measuring 1.5 meters by 1.5 meters square was dug
on the site of black clay to a depth of 2.5 meters, surpassing the grey and the black sheets of soils. On this site the grey sheet lies on top of the black one. Using a spade and a shovel about 20 kg of the black soil from the black sheet was excavated from the sides of
the pit. Similarly about 20 kg of the grey clay was excavated from its sheet.
The brown clay was removed from its marked site on the one acre square valley. A pit of about 1.5 meters by 1.5 meters square was dug using a shovel and spade up to a depth of about 1.5 meters. About 20 kg of brown soil was excavated using a shovel from the sides
of the pit (Hesse, 1971).
The wet black, brown and grey clay soil samples and about 20 kgs of the Ilesi potters mixture were wrapped into clear polythene papers for transportation.
3.3 Pretreatment of samples
The wet clay samples collected from Ilesi deposits were broken by hand into small lumps
3.3.1 Pretreatment for chemical characterization
Approximately 50g of each of the black, brown and grey dry clay samples were crushed using a wooden hammer. The crushed samples were sieved on 0.425 mm sieve and stored in clear polythene papers for the following spectroscopic analysis.
i) FTIR in which the infrared spectra were recorded on Nicolet Avatar 320 FTIR
spectrometer, equipped with DTGS KBr detector. ii) XRD was done on a Bruker XRD D2 Phaser.
iii) The clays were analyzed for their elemental composition by using a Shimadzu
Ray EDX-800 HS.
The samples were used in chemical characterization as follows:
126.96.36.199 FTIR analysis
KBr pressed disc technique was used for preparing approximately 2g of the crushed clay solid sample. The 2g sample was put into the cell holder and inserted into the spectrometer. The spectrometer produced absorption and transmittance spectra for each
188.8.131.52 XRD analysis
Approximately 2g sample was re-crushed into very fine powder then put into the cell holder and inserted into the spectrometer. The spectrometer produced diffractograms for each clay. The spectrometer’s computer analyzed the difractrograms into percentage
184.108.40.206 EDX analysis
Approximately 2g sample was put into the cell holder and inserted into the EDX spectrometer. The spectrometer produced spectra for each clay. The spectrometer’s
computer analyzed the spectra into percentage elements as oxides.
3.3.2 Pretreatment for physical characterization
Approximately 500g of each of the clays namely, the black, brown and grey clays were crushed using a wooden hammer. The crushed samples were sieved on 0.425 mm sieve and stored in clear polythene bags for Atterberg limits determinations, loss on ignition
and moisture content. Approximately 350g of dry clay lumps were put aside for the particle size test.
The remaining dry lumps of clay samples were crushed by KUD- Humboldt-Wedaq and
sieved on 2 mm standard mesh in order to remove the gravel, rock and organic matter like humus, roots and stems. The soil that passed through the sieve was milled using Marina Torrential Super. The soil samples from the mill were sieved on 0.425 mm mesh
and stored in dry polythene paper bags for determination of physical parameters of shrinkage, density, porosity and compressive strengths. Samples used in the
determination of these physical properties were either cured or uncured. They were categorized as follows:
i) Uncured sieved raw clays were the black, brown, R1 and grey clays that were molded
to plasticity and subjected to physical tests immediately.
ii) Cured sieved raw clays were clays and mixtures R2-R5 that were covered into plastic
3.4 Physical parameter determination
The physical properties of the cured and uncured clay bodies of black, brown, grey were
tested to determine the suitability of the raw clays and formulate recipes.
3.4.1 Determination of Atterberg limits
220.127.116.11 Liquid limit (ASTM D 4318)
This was done by the Cone Penetrometer Test (Rogers, 2006). Approximately 200g of the dry milled and sieved black sample was mixed with water on a flat glass plate using two metallic spatulas until plastic. A metallic cup was inverted and pressed into the
molded sample hip. This was done carefully such as not to allow air into the sample. The cup with the wet clay was turned upright. A metallic spatula was used to level the clay in
the cup. The metallic cup with the black clay body was put under the cone penetrometer. The cone was adjusted to the level of the clay in the cup. The gauge pointer was then adjusted to zero. The cone was released into the clay by pressing cone release button. The
dial gauge was then adjusted to join the joining rod. A reading by the dial gauge when the rods join was recorded to give the penetration. The cone was removed and cleaned using
damp piece of cloth. Approximately 35g of the sample from around the penetration region was removed from metallic cup. Approximately 5g from the 35g was set aside for the plastic limit determination while the remaining was put into another metallic cup and
weighed as WM. The cup with approximately 30g sample was taken into an oven and dried for 24 hours at 110°C. It was removed after the 24 hours and weighed as DM. The
%Moisture content = equation (4)
where WM is Wet mass and DM, Dried mass.
The remaining sample on the mixing glass surface was adjusted using water or dry
sample to achieve a penetration of between 15 and 22 mm. This test was repeated four times. At each penetration test, moisture content of the sample was determined by using equation (4) above. A graph of each penetration against its percentage moisture was
plotted. This test was repeated for the brown and grey clay molds. Liquid limit was calibrated as percentage moisture at 20 mm penetration for each of the black, brown and
grey clay bodies.
18.104.22.168 Plastic limit (ASTM D 4318)
The approximately 5g of the black clay body set aside in cone penetrometer test above was prepared for the plastic limit determination by adding dry sample powder or water
until a desired plasticity. It was rolled into a thread of about 3mm in diameter on the glass plate it did not break into pieces. Small portions dry black clay soil were added to it and rolled again into threads of about 3mm until the pieces cracked. The cracked pieces were
transferred into a metallic cup weighed as WM and then kept in an oven at 110°C for 24 hours to dry. The dry sample was weighed as DW. This was repeated 3 times. The plastic
3.4.2 Particle size analysis
Approximately 350g of the 0.425mm crushed and sieved black clay sample was poured on a glass plate. Rocks and organic matter were removed by hand picking (Klinefelter and Hamlin, 1957). Approximately 250g of the remaining sample was shaken through a
stack of registered sieves of 2mm, 1mm, 0.6mm, 0.425mm, 0.3mm, 0.212mm and 0.15mm using an electric shaker (Abolarin et al., 2006; Barsom, 2003). The masses
remaining on sieves 0.212 mm, 0.3mm, 0.425mm, 0.6mm, 1.0mm and 2 mm were taken and weighed to determine percent silt and sand by sieve analysis, ASTM D422. This was repeated for the brown and grey clay powders.
The sieved sample that passed through 0.212 mm sieve was analyzed for the clay content
by the hydrometer ASTM 152H. This sample was mixed with 125 ml of 25% sodium hexametaphosphate solution, prepared by dissolving 40g sodium hexametaphosphate in
1000mL distilled water, to deflocculate the clay particles. The pretreated soil mixture was transferred into a 1000mL control cylinder and filled to the mark using deionized water. The hydrometer was dipped into the control/blank prepared by mixing 125 mL dispersing
agent with deionized water to make 1000 mL solution. After reading the zero, the hydrometer was transferred into the sample placed in a 1000 mL cylinder. The meniscus
level of the hydrometer was read after 30 seconds to give the clay and silt proportions. The hydrometer readings were repeated at 1, 2, 4, 8, 15, 30, 60, 120, 240 and 1440 minutes. The data collected was used to draw a graph from which the percent clay and
3.4.3 Loss on ignition
Exactly 25g of milled and sieved black clay was dried in an oven at 110°C for 12 hours and put into a pre-weighed crucible, M6 and weighed, M4. The sample and crucible were heated in a kiln at 600°C for 6 hrs to burn out all carbon content. The sample was then
cooled in a dessicator overnight to avoid absorption of moisture and weighed. Its mass was given as, M5. The loss on ignition was calculated using equation (5) below. The
procedure was repeated for the black clay at 800°C, and 1000°C, and for the brown and grey clays at 600°C, 800°C, and 1000°C to determine their carbon contents at varying calcinations temperatures.
Loss on ignition = x 100 equation (5)
3.4.4 Moisture content
Three clay blocks measuring 40mm long by 20mm wide by 20mm high were baked from molded uncured black clay. The blocks were put on pieces of aluminium paper and
weighed to give wet weight as WW. They were dried in air for three weeks and in an oven for 24 hours at 110°C. The pieces were removed and immediately weighed with the
aluminium paper to give dry weight as DW. The percentage moisture was calculated from equation (6) below.
3.4.5 Shrinkage limits
Three blocks measuring 140mm long by 20mm wide and 20mm height were baked from the uncured black clay that had been molded to plasticity. Their lengths recorded as 140 mm. The pieces were left in the molding blocks for four days to dry. They were then
removed and dried in air for two weeks. The pieces were then dried in the oven for 24 hrs at 110°C. Their lengths were measured and recorded as dry length, DL. They were fired
in an oven at 600°C for six hrs and allowed to cool in the kiln. Their lengths were then measured in mm as Fired length, FL (Allen, 1986). The percentage shrinkage was calculated from the equations (7) and (8) below.
% Linear dry shrinkage = Equation (7)
% Linear fired shrinkage = Equation (8)
This procedure was repeated for the uncured black clay body at 800°Cand 1000°C. It was also repeated on similar blocks of uncured brown, uncured grey, potters mixture R1,cured black, cured brown, cured grey at 600° C, 800°Cand 1000°C.
Twelve blocks measuring 40mm long by 20mm wide and 20mm height were molded from the uncured black clay. They were dried in air for two weeks, then in oven for 12
hours at 110°C. Three of the pieces were used to determine dry density. Each piece was weighed and immersed into kerosene in an overflow can. The volume of the displaced
blocks fired at 800°Cand the last three fired at 1000°C. The procedure above was repeated for similar blocks of uncured brown, uncured grey, R1, cured black, cured brown and
cured grey clays at 600°C, 800°C and 1000°C.
The porosity of fired clay bodies was determined by Water Evaporation Method, WEM.
Nine blocks measuring 40mm long by 20mm wide and 20mm height were baked from molded uncured black clay. The pieces were left to dry in the molding blocks for one week. They were removed and left to dry in air for another one week. They were then
dried for 24 hours in an oven at 110°C. Three of the bone dry blocks were fired in a kiln to temperatures of 600°C, cooled in the oven at 110° C for 2 hrs after which they were
transferred into desiccators to cool to room temperature. They were weighed as dry weight, WD. The three blocks were then boiled in water for half an hour, and then left
soaked into the cold water for 15 hrs. They were removed from the water and wiped dry using a damp towel and weighed to get the wet weight, WW. Porosity was determined as percentage water absorbed using the equation (9) below.
Porosity = x 100 Equation (9)
The above procedure was repeated on three blocks fired at 800°C and another three blocks kilned to 1000°C. Their porosities were determined using the equation (9).This
3.4.8 Compressive strengths
The green and fired compressive strengths of clay product were measured as fracture load (Klinefelter and Hamlin, 1957). Twelve blocks measuring 40mm long by 40mm wide and 40 mm height were made from the uncured black clay mold. The blocks were left in the
molding blocks for one week to dry. They were then removed and dried for two weeks in air. The pieces were dried in the oven for 24 hrs at 110° C. The dry pieces were then
subjected to fracture load using Universal compression and bending machine. Three other blocks were fired to 600°C in a kiln, cooled and subjected fracture load. Three others were fired to 800°C and subjected to fracture load. The last three were fired to 1000°C
and subjected to fracture load. This procedure was repeated for the uncured brown, uncured grey, R1, cured black, cured brown and cured grey at green, 600°C, 800°C and
3.5 Recipe formulation
After chemical and physical characterization of the black, brown, grey clays and R1, a recipe used by Ilesi potters, mixtures R2 to R6 were developed by mixing the raw clays
in optimized ratios. Quantities by percentage ratios of raw materials were measured accurately as shown in Table 3.1. A total of 5 kg of each mixture was molded to
plasticity. For instance R2 was prepared by weighing 1000g black sieved clay, 1500g brown sieved, 1500g grey sieved and 1000g sieved grog sand. The masses for the ratios in R3 to R6 were determined in a similar manner. These mixtures were kept in polythene
Table 3.1: Ratios of percentage raw materials by mass
Material used Recipe
R 1 R 2 R 3 R 4 R 5 R 6
% Black clay Approx.28 20 15 20 20 25 % Brown clay Approx.28 30 20 30 40 30 % Grey clay Approx.28 30 35 30 30 30
% Grog Approx.16 20 30 0 5 15
% SCBA 0 0 0 20 5 0
% Total 100 100 100 100 100 100
SCBA is Sugar cane Bagasse Ash
These recipe formulations, R2 to R6 were tested on the physical parameters of shrinkage,
density, porosity and compressive strength so as to establish the recipe that is most suitable for pottery.
3.5.1 Shrinkage limits
Three blocks measuring 140mm long by 20mm wide and 20mm height were molded to plasticity from R2. Their lengths recorded as 140 mm. The pieces were left in the molding blocks for four days to dry. They were then removed and dried in air for two
weeks. The pieces were then dried in the oven for 24 hrs at 110°C. Their lengths were measured as dry length, DL. They were fired in an oven at 600°C for six hrs and allowed
to cool in the kiln. Their lengths were then measured in mm as Fired length, FL (Allen, 1986). The percentage shrinkage was calculated from the equations (7) and (8) on page 27. This procedure was repeated for the R3, R4, R5 and R6 at 600°C. The shrinkage of
R2, R3, R4, R5 and R6 was determined in the same manner at 800°Cand 1000°C.
Twelve blocks measuring 40mm long by 20mm wide and 20mm height were molded
110°C. Three of the pieces were used to determine dry density. Each piece was weighed and immersed into kerosene in an overflow can. The volume of the displaced kerosene
was measured. Three pieces were fired in a kiln at 600°C. They were transferred and cooled in the oven. Each of the pieces was weighed and its density determined using
water in the overflow can. This procedure was repeated on 3 blocks fired at 800°C and the last three fired at 1000°C. The procedure above was repeated for similar blocks of R2, R3, R4, R5 and R6 at 600°C, 800°C and 1000°C.
Nine blocks measuring 40mm long by 20mm wide and 20mm height were baked from molded R2. The pieces were left to dry in the molding blocks for one week. They were
removed and left to dry in air for another one week. They were then dried for 24 hours in an oven at 110°C. Three of the bone dry blocks were fired in a kiln to temperatures of
600°C, cooled in the oven at 110° C for 2 hrs. They were then transferred into desiccators to cool to room temperature and weighed, WD. The three blocks were then boiled in water for half an hour, and then left soaked into the cold water for 15 hrs. They were
removed from the water and wiped dry using a damp towel and weighed, WW. Porosity was determined as percentage water absorbed using the equation (9) on page 28. This
procedure was repeated on three blocks of R2 fired at 800°C and another three blocks kilned to 1000°C. Their porosities were determined using the equation (6) on page 26. The procedure above was repeated for similar blocks of R3, R4, R5 and R6 at 600°C,
3.5.4 Compressive strengths
Twelve blocks measuring 40mm long by 40mm long and 40 mm height were made from R2. The blocks were left in the molding blocks for one week to dry. They were then removed and dried for two weeks in air. The pieces were dried in the oven for 24 hrs at
110° C. Three of the dry pieces were then subjected to fracture load using Universal compression and bending machine. Three other blocks were fired to 600°C in a kiln,
cooled and subjected fracture load. Three were fired to 800°C and subjected to fracture load. The last three were fired to 1000°C and subjected to fracture load. The procedure above was repeated for similar blocks of R2, R3, R4, R5 and R6 at 600°C, 800°C and
Losses were determined by identifying the number of blocks that showed swelling during
forming and those that cracked during drying and firing during the shrinkage tests.
Uncured black clay was molded to plasticity. The clay body was gently pressed into the
shrinkage molding blocks placed on a flat table to form twelve 140mm long by 20mm wide and 20mm height blocks. The top of the mold for each sample was leveled using a metallic plate. The number of wet clay blocks that showed swelling on top were marked
Twelve blocks of the uncured black clay body measuring 140mm long by 40mm wide
and 40mm height were prepared in the shrinkage wooden blocks and allowed to dry in air for 4 days. They were removed and dried in air for one week. They were put in an oven at
110°C for 24 hours. Those that showed cracking after being removed from the oven were counted and recorded. This was repeated for the uncured brown, R1, uncured grey, cured black, cured brown, cured grey clay bodies, R2, R3, R4, R5 and R6.
Twelve blocks of the uncured black measuring 140mm long by 40mm wide and 40mm
height were prepared in the shrinkage wooden blocks and allowed to dry in air for 4 days. They were removed and dried in air for one week. They were put in an oven at 110°C for 24 hours. They were fired in a kiln at 600°C. The blocks of the clay bodies that cracked
were counted and recorded. This was repeated at 800°C and 1000°C noting the number that cracked at each firing temperature. This was repeated for the uncured brown, R1,
uncured grey, cured black, cured brown, cured grey clay bodies, R2, R3, R4, R5 and R6 at firing temperatures of 600°C, 800°C and 1000°C.
3.7 Data analysis
Atterberg limits data and sieve analysis were analyzed by regression analysis with linear
4 RESULTS AND DISCUSSION 4.1 Introduction
This study set out to determine the physical and chemical characteristics of the raw clays
used for pottery by Ilesi potters. Three soil samples coloured black, brown and grey were collected and each was divided into two. One set was used without curing while the other was cured for 21 days before use for physical characterization. To gain insight into the
causes of the losses incurred by the Ilesi potters, the soil samples and grog were mixed in different ratios (R2 to R6) and molded into blocks whose physical properties were
determined and compared with those made from the recipe use by Ilesi potters, R1 (Table 4.1). Results on the physical properties of the cured and uncured black, brown and grey clays, Atterberg limits, particle size, loss on ignition, moisture content, shrinkage,
compressive strengths, porosity and density are presented and discussed.
Table 4.1: Sample groups
1 2 3 4 5 6 7 8 9 10 11 12
Uncured black Cured black Uncured brown Cured brown Uncured grey Cured grey
R1 R2 R3 R4 R5 R6
The data on mineralogy and elemental composition of the clays is presented in tables, spectra and compared with results obtained in studies from other areas.
4.2 Screening tests of raw clays
The black clay soil was found to be more uniform and rigid, with very few sand particles
little crystalline particles. The brown and grey samples had coarse particles, transparent pieces of rock attributed to the high percent microcline at 42.6% and 44.6% respectively
as seen in table 4.4. Both had a crystalline feel. Table 4.2 gives the soil profile of the clay deposits, their appearances and compositions in terms of percentage clay, silt and sand
from the sieve analysis as in table 4.7.
Table 4.2: Profile description of clay soils from deposit depths when milled
Depth/m Sample Description % Clay+ silt % Sand
0.5-1.0 Grey Dark-grey coarse, crystalline particles, humus, wooden sticks.
1.0-1.5 Brown Reddish brown in grey, rough surface, transparent coarse, crystalline particles.
1.2-2.0 Black Black, smooth and stone hard, fine powder.
4.3 Mineral and chemical composition of raw clays
The mineral composition of each of the three types of clays studied were determined by
FTIR and correlated by powder x-ray diffraction. The chemical composition of the clays was determined by EDX and the results are presented and discussed below.
4.3.1 FTIR Spectroscopy
As the individual clays often occur in a form of mixed-layer clay minerals with various ratios of individual components, IR curves were recorded to confirm the clay mineral
print region representing Si-O and Al-OH stretching respectively (Tan, 2011). The spectrum for black clay is given in figure 4.1 below.
Figure 4.1: FTIR spectrum for black clay
The bands at 3693.4 cm-1 and 3622.1 cm-1 in figure 4.1 are attributable to the octahedral OH stretching in dickite. The bands at 1029.9 cm-1, 788.8 cm-1, 688.5 cm-1 in the
fingerprint region could be due to the tetrahedral Si-O-Si and Si-O stretching while the peaks at 540.0 cm-1 and 468.7 cm-1 can be attributed to the Si-O deformation (Abuh et al.,
2014). Figure 4.2 shows the FTIR spectrum of the brown clay.
The bands at 3693.4 cm-1 and 3622.1 cm-1 in figure 4.2 are attributable to the octahedral OH stretching in the dickite. The bands at 1031.8 cm-1,783.0 cm-1, 690.5 cm-1 in the
fingerprint region could be due to the tetrahedral Si-O-Si and Si-O stretching. The bands 536.2 cm-1 and 466.7 cm-1 could be due to the Si-O deformation. The band seen at 914.2
cm-1 in the fingerprint region can be attributed to the octahedral Al-O-H stretching. Figure 4.3 shows the FTIR spectrum of the grey clay.
Figure 4.3: FTIR spectrum for grey clay
The grey clay in figure 4.3 has peaks seen at 3435.0 cm-1 and 1651 cm-1that can be assigned to the H-O-H stretch of free water or water bound by hydrogen bonding. The bands at 3693.4 cm-1 and 3622.1 cm-1 may be due to the octahedral OH stretching in the
dickite with the band at 1031.8 cm-1 in the fingerprint region being for the Al-O-H stretching. The bands at 1031.8 cm-1, 781.1 cm-1, 690.5 cm-1 in the fingerprint region can
be attributed to the tetrahedral Si-O-Si and Si-O stretching. The bands at 536.2 cm-1 and 466.7 cm-1are attributed to Si-O deformation. The spectra for the black, brown and grey clays are similar and their analysis point to a sample of a clay mineral with dickite, alkali
The IR spectra of kaolins showed a doublet at 3696 cm-1 and 3620 cm-1. The doublet at
3693.4 cm-1 and 3622.1 cm-1 in figures 4.1, 4.2 and 4.3 can then be attributed to dickite Al-O-H stretching whose fingerprint region showed bands for the same stretching at
1029.9 cm-1 in figure 4.1 and 1031.8 cm-1 in figures 4.2 and 4.3. In baseline studies on kaolinite FTIR bands were seen at 3694 cm-1, 3620cm-1 and 1033 cm-1 (Jana and Peter, 2001). These bands are similar to the peaks obtained for the Ilesi clays.
22.214.171.124 Albite and Microcline
Feldspars have fingerprint region in 1150-1000 cm-1. Therefore the bands at 1031.8cm-1 in figures 4.5 and 4.6 and 1029.9 cm-1 in figure 4.4 are then attributed to Si-O-Si stretching. The bands at 690.5 cm-1 in figures 4.2 and 4.6, 688.5 cm-1 in figure 4.1, 540.0
cm-1 in figure 4.1, 536.2 cm-1 in figures 4.2 and 4.3 confirm Si-O-Al stretching in the feldspars. These spectra are similar to those of the research on central Bosnia clays
(Jovanovic and Mujkanovic, 2013).
Quartz has fingerprint bands at 1100 cm-1, 800 cm-1, 500 cm-1. Therefore the bands at
1031.8 cm-1 in figures 4.2 and 4.3, 1029.9 cm-1 in figure 4.4 are therefore attributed to Si-O-Si stretching. The bands at 788.8 cm-1 in figure 4.1, 783 cm-1 in figure 4.5 and 781.1
comparison of spectral bands for the Ilesi clays alongside those recorded in a different research (Preeti and Singh, 2007).
Table 4.3: Spectral bands and their assignments
Black/cm-1 Brown / cm-1 Grey/cm-1 Preeti’s Clay/ cm-1 Assignments 3693.4 3693.4 3693.4 3696.7 Al-O-H stretching
3622.1 3622.1 3622.1 3622.5 Al-O-H (inter octahedral) stretching 3438.8 3440.8 3435.0 3450.4 H-O-H stretching
1651 1651.0 1651.0 1633.4 H-O-H stretching
1029.9 1031.8 1031.8 1033.3 Si-O-Si stretching, Si-O-, stretching 914.2 914.2 914.2 914.5 Al-O-H, stretching
788.8 783.0 781.1 790.9 Si-O-, stretch., Si-O-Al, Si-O-(Mg,Al stretching
688.5 690.5 690.5 693.4 Si-O-, stretching Si-O-Al, stretching 540.0 536.2 536.2 538.4 Si-O-, stretching Si-O-Al, stretching 468.7 466.7 466.7 468.9 Si-O- stretching, Si-O-Fe stretching
4.3.2 X-Ray Diffraction (XRD)
It shows that the clays analyzed contained dickite, Al4Si4O10 (OH)8, albite, NaAlSi3O10,
microcline, KAlSi3O8, and quartz, SiO2 as shown in table 4.4.
Table 4.4: XRD data for the clay samples
Clay name %Albite % Dickite %Microcline %Quartz
Black 22.4 15.8 38.2 23.6
Brown 16.1 6.4 42.6 34.8
Grey 15.6 7.3 44.6 32.5
The clay soils analyzed had the same mineral assemblage since they were removed from the same valley. Albite and microcline are alkali feldspar fluxes while quartz is filler as
well as a glassing material in pottery production. The results showed that the black clay has the highest percentage dickite and albite content of 15.8%, and 22.4%, respectively.
and grey clays. However, the physical properties of raw clays make it necessary to have the clays mixed into mixtures (Kent, 2008). For example, this black clay was sticky and
difficult to achieve plasticity. XRD’s diffracted x-ray beam from the clay sample is detected as a characteristic x-ray line on photographic plates whose intensity registers as
peaks against their phase angle (Katherine and Benjamin, 1996). Figure 4.4 shows the diffractogram of the black clay.
Figure 4.4:X-Ray Diffractogram for black clay
Key:d represents dickite, a , albite, m, microcline and q, quartz.
Kaolinite exhibits a characteristic first order diffraction peak at 2θ, 12.4°corresponding to a spacing of 0.713 nm and a second order diffraction at 2θ, 25° corresponding to a
0.630-0.645 nm and 0.310-0.325 nm (Tan, 2011) and quartz. Figure 4.5 shows the diffractogram for the brown clay.
Figure 4.5: X-Ray diffractogram for brown clay soil
Key: d represents dickite, a, albite, m, microcline and q, quartz.
Like in the black clay, peaks identified in figure 4.5 are for dickite, quartz, albite and microcline. This shows that the mineral assemblage in brown clay is the same as in black
Figure 4.6: X-Ray Diffractogram for grey clay
Key: d represents dickite, a, albite, m, microcline and q, quartz.
The peaks for grey clay in figure 4.6 were at the same phase angles as in the black and brown showing presence of dickite, quartz, albite and microcline.
Generally figures 4.4, 4.5 and 4.6 showed dickite peaks are at 2θ, 12.4° and 21.5°, albite at 2θ, 22° and 28°, microcline at 2θ, 27.4° and 35° while quartz at 2θ, 21° and 26.9°
degree of crystallinity that causes mutual interference with the diffraction patterns analysis (Ronald, 1967).
The data showed that iron is not in the clays as a mineral which would mean that all the
iron in the clay body is lying in the interlayer distances as accessory ion. On average the accessory minerals are in very small percentages to show on diffractograms. The Ilesi clay mineralogy results are similar with those of other deposits like research on
mineralogy of local clays in a Saudi Arabia (Mohsen and El-maghraby, 2010) and that done on central Bosnia clays (Jovanovic and Mujkanovic, 2013).
4.3.3 EDX spectroscopy
The results of element analysis as oxides are shown in the table 4.5. Table 4.5: Percentage oxides of raw materials
% Elements Black ±SE Brown ±SE Grey ±SE Sand ±SE
SiO2 64.94±0.614 63.86±0.607 67.50±0.557 51.18±0.684 Al2O3 20.70±0.822 21.48±0.846 19.67±0.732 24.20±1.102 Fe2O3 7.56±0.034 7.40±0.034 4.76±0.026 16.49±0.057 K2O 2.91±0.028 5.92±0.037 4.80±0.031 3.73±0.035 CaO 1.49±0.018 0.23±0.050 1.07±0.015 1.36±0.021 TiO2 1.42±0.033 1.04±0.030 1.26±0.032 1.62±0.039 SO3 0.91±0.047 0.00 0.64±0.033 1.00±0.051 SrO 0.05±0.001 0.05±0.001 0.04±0.001 0.10±0.002 Rb2O 0.02±0.001 0.03±0.001 0.03±0.001 0.050±0.002
N.B: mean±sd (n = 3), black=Ilesi black, brown= Ilesi brown, Grey =Ilesi grey.
Table 4.5 shows that the major components in the samples were SiO2, Al2O3 and Fe2O3. The SiO2 composition ranged between 63.86%-67.5%, Al2O3, 19.67%-21.48% and
Fe2O3, 4.76%-7.56%. This data is similar to research on chemical composition of different clays and pure kaolin in Saudi Arabia (Mohsen and El-Maghraly, 2010),
Nigeria (Abuh et al., 2004), clays in Odupani in South eastern Nigeria (Osabar et al., 2009).
The percentage of MgO is below detection level. These clays should not expand during
drying which can cause cracking (Kirk and Othmer, 2004). The percentage of CaO from table 4.5 is low, that is between 0.23±0.050% and 1.49±0.018% which suggests that these clays should not have swelling properties (Kirk and Othmer, 2004). This rules out the
nature of the clays being responsible for the cracking during drying and firing by the potters at Ilesi. This is confirmed by the XRD data from table 4.4 that shows absence of
bentonites, calcite and dolomite.
Although the clays are missing Na2O, the percentage composition of albite in table 4.4
serves well for glass formation during the firing process. The data on table 4.5 also shows a ratio of silica: alumina to be 3:1 (Folorunso et al., 2014) for the black, brown and grey
clays suggesting that these clays can also be used to manufacture synthetic zeolite (Nwosu, 2013).
Iron (III) oxide at 7.56%, 7.4%, 4.76% and 16.49% in black, brown, grey and sand respectively gives red colour to fired pots especially in those mixtures with high
percentage of the brown clays. In addition they also act as fluxes during the sintering process. These iron (III) oxide levels are however too high for high quality ceramic products like bathroom tiles that require below 1% iron oxide (Olale, 1985). If a wet
the clay would reduce the percentage of this iron and other elements like calcium and titanium making it suitable for production of these tiles (Karoki, 2008).
The amount of K2O is higher in the grey, 4.8%, than the black, 2.91%, due to the higher
percentage microcline feldspar, 44.6% as seen in table 4.2 which yields the free K2O during the hydrothermal alteration according to the equation (1) on page 5.
4.4 The Physical Properties of the Ilesi Clays
The properties determined in this study include plasticity index, particle size, loss on
ignition, moisture content, linear shrinkage, densities, porosity and compressive strengths.
4.4.1 Plasticity index
It was generally recognized that fall cone tests were difficult to perform at water contents near the plastic limit since the soil samples are stiff and difficult to mix (Feng, 2000; Stone and Phan, 1995). Figure 4.7 shows the best of fit lines from these penetrometer
Figure 4.7: Penetration against moisture content for the black, brown and grey clays
The liquid limits are calculated from the line equations in figure 4.7 at mean
penetrometer value of 20mm as follows:
Black clay Brown clay Grey clay
Y= -69.94+1.9x 1.9x=20+69.94 X = 47.34%
y = -51.96+1.92x 1.92x =20+51.96 x = 37.48%
y=-1.2x102+4.51x 4.51x =20 + 120 x = 31.04%
Table 4.6 shows the plasticity index (PI) values. Table 4.6: Atterberg limits for the black, brown and grey soils
Clay soil BLACK GREY BROWN
Liquid Limit(% L.L) 47.34 31.04 37.48
Plastic Limit% (PL) 28.80 21.50 20.00